#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/16/4341657.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4341657
loop_
_publ_author_name
'Treadwell, LaRico J'
'Watkins-Curry, Pilanda'
'McAlpin, Jacob D.'
'Rebar, Drew J.'
'Hebert, Jessica K.'
'DiTusa, John F.'
'Chan, Julia Y.'
_publ_section_title
;
 Investigation of Mn, Fe, and Ni Incorporation in CeCo2Al8.
;
_journal_issue                   3
_journal_name_full               'Inorganic chemistry'
_journal_page_first              963
_journal_page_last               968
_journal_paper_doi               10.1021/ic502356t
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'Al8 Ce Co1.30 Fe0.70'
_chemical_formula_sum            'Al8 Ce Co1.3 Fe0.7'
_chemical_formula_weight         469.83
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           55
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2014-09-13 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.4990(5)
_cell_length_b                   14.4100(5)
_cell_length_c                   4.0340(5)
_cell_measurement_temperature    293(2)
_cell_volume                     726.57(10)
_computing_cell_refinement       'Denzo and Scalepack (Otwinski & Minor 1997)'
_computing_data_collection       'Collect (Nonius 1999)'
_computing_data_reduction        'Denzo and Scalepack (Otwinski & Minor 1997)'
_computing_molecular_graphics    'Crystal Maker'
_computing_publication_material  Publcif
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'Direct Methods, SIR 97'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Nonius Kappa CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0278
_diffrn_reflns_av_sigmaI/netI    0.0319
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            2231
_diffrn_reflns_theta_full        30.99
_diffrn_reflns_theta_max         30.99
_diffrn_reflns_theta_min         2.83
_exptl_absorpt_coefficient_mu    10.990
_exptl_absorpt_correction_T_max  0.794
_exptl_absorpt_correction_T_min  0.667
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'HKL scalepack (Otwinski & Minor, 1997)'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.295
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Fragment
_exptl_crystal_F_000             856
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.465
_refine_diff_density_min         -1.121
_refine_diff_density_rms         0.239
_refine_ls_extinction_coef       0.0019(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.091
_refine_ls_matrix_type           full
_refine_ls_number_parameters     72
_refine_ls_number_reflns         1303
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.091
_refine_ls_R_factor_all          0.0385
_refine_ls_R_factor_gt           0.0263
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0247P)²+1.2367P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0562
_refine_ls_wR_factor_ref         0.0610
_reflns_number_gt                1054
_reflns_number_total             1303
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            ic502356t_si_008.cif
_cod_data_source_block           shelxl
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4341656--4341665.cif.
;
_cod_original_sg_symbol_H-M      Pbam
_cod_original_formula_sum        'Al8 Ce Co1.30 Fe0.70'
_cod_database_code               4341657
#BEGIN Tags that were not found in dictionaries:
_exptl_crystal_f_000'            866.81
#END Tags that were not found in dictionaries
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x+1/2, -y+1/2, -z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'-x-1/2, y-1/2, z'
'x-1/2, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ce1 Ce 0.34069(2) 0.318403(18) 0.0000 0.01090(10) Uani 1 2 d S
Co1 Co 0.03426(5) 0.40701(4) 0.0000 0.0091(2) Uani 0.48(3) 2 d SP
Mn1 Mn 0.03426(5) 0.40701(4) 0.0000 0.0091(2) Uani 0.52(3) 2 d SP
Co2 Co 0.15077(5) 0.09698(4) 0.0000 0.0079(2) Uani 0.83(3) 2 d SP
Mn2 Mn 0.15077(5) 0.09698(4) 0.0000 0.0079(2) Uani 0.17(3) 2 d SP
Al1 Al 0.02544(12) 0.13168(10) 0.5000 0.0102(3) Uani 1 2 d S
Al2 Al 0.15965(11) 0.37890(10) 0.5000 0.0098(3) Uani 1 2 d S
Al3 Al 0.23536(12) 0.17282(10) 0.5000 0.0110(3) Uani 1 2 d S
Al4 Al 0.33181(12) 0.49169(10) 0.5000 0.0105(3) Uani 1 2 d S
Al5 Al 0.45247(11) 0.18000(9) 0.5000 0.0103(3) Uani 1 2 d S
Al6 Al 0.09526(11) 0.25321(9) 0.0000 0.0107(3) Uani 1 2 d S
Al7 Al 0.33812(11) 0.04485(10) 0.0000 0.0119(3) Uani 1 2 d S
Al8 Al 0.0000 0.5000 0.5000 0.0105(4) Uani 1 4 d S
Al9 Al 0.0000 0.0000 0.0000 0.0104(4) Uani 1 4 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al1 Ce1 Al1 79.65(4) 3_556 3
Al1 Ce1 Al2 150.75(4) 3_556 1_554
Al1 Ce1 Al2 93.06(3) 3 1_554
Al1 Ce1 Al2 93.06(3) 3_556 .
Al1 Ce1 Al2 150.75(4) 3 .
Al2 Ce1 Al2 79.51(3) 1_554 .
Al1 Ce1 Al5 53.95(3) 3_556 .
Al1 Ce1 Al5 103.21(3) 3 .
Al2 Ce1 Al5 154.06(4) 1_554 .
Al2 Ce1 Al5 94.78(3) . .
Al1 Ce1 Al5 103.21(3) 3_556 1_554
Al1 Ce1 Al5 53.95(3) 3 1_554
Al2 Ce1 Al5 94.78(3) 1_554 1_554
Al2 Ce1 Al5 154.06(4) . 1_554
Al5 Ce1 Al5 79.27(3) . 1_554
Al1 Ce1 Al3 148.94(4) 3_556 1_554
Al1 Ce1 Al3 92.74(3) 3 1_554
Al2 Ce1 Al3 58.80(3) 1_554 1_554
Al2 Ce1 Al3 106.84(3) . 1_554
Al5 Ce1 Al3 99.83(3) . 1_554
Al5 Ce1 Al3 50.58(4) 1_554 1_554
Al1 Ce1 Al3 92.74(3) 3_556 .
Al1 Ce1 Al3 148.94(4) 3 .
Al2 Ce1 Al3 106.84(3) 1_554 .
Al2 Ce1 Al3 58.80(3) . .
Al5 Ce1 Al3 50.58(4) . .
Al5 Ce1 Al3 99.83(3) 1_554 .
Al3 Ce1 Al3 78.32(3) 1_554 .
Al1 Ce1 Al6 140.173(18) 3_556 .
Al1 Ce1 Al6 140.173(18) 3 .
Al2 Ce1 Al6 52.77(3) 1_554 .
Al2 Ce1 Al6 52.77(3) . .
Al5 Ce1 Al6 103.76(3) . .
Al5 Ce1 Al6 103.76(3) 1_554 .
Al3 Ce1 Al6 54.10(3) 1_554 .
Al3 Ce1 Al6 54.10(3) . .
Al1 Ce1 Al4 56.33(4) 3_556 .
Al1 Ce1 Al4 104.48(3) 3 .
Al2 Ce1 Al4 99.32(3) 1_554 .
Al2 Ce1 Al4 50.12(4) . .
Al5 Ce1 Al4 96.03(3) . .
Al5 Ce1 Al4 154.99(4) 1_554 .
Al3 Ce1 Al4 153.25(4) 1_554 .
Al3 Ce1 Al4 95.73(3) . .
Al6 Ce1 Al4 101.22(3) . .
Al1 Ce1 Al4 104.48(3) 3_556 1_554
Al1 Ce1 Al4 56.33(4) 3 1_554
Al2 Ce1 Al4 50.12(4) 1_554 1_554
Al2 Ce1 Al4 99.32(3) . 1_554
Al5 Ce1 Al4 154.99(4) . 1_554
Al5 Ce1 Al4 96.03(3) 1_554 1_554
Al3 Ce1 Al4 95.73(3) 1_554 1_554
Al3 Ce1 Al4 153.25(4) . 1_554
Al6 Ce1 Al4 101.22(3) . 1_554
Al4 Ce1 Al4 77.81(3) . 1_554
Al1 Ce1 Al9 51.26(2) 3_556 3
Al1 Ce1 Al9 51.26(2) 3 3
Al2 Ce1 Al9 102.39(3) 1_554 3
Al2 Ce1 Al9 102.39(3) . 3
Al5 Ce1 Al9 103.56(3) . 3
Al5 Ce1 Al9 103.56(3) 1_554 3
Al3 Ce1 Al9 140.557(17) 1_554 3
Al3 Ce1 Al9 140.557(17) . 3
Al6 Ce1 Al9 144.30(3) . 3
Al4 Ce1 Al9 53.29(2) . 3
Al4 Ce1 Al9 53.29(2) 1_554 3
Al6 Co1 Al8 124.884(13) . .
Al6 Co1 Al8 124.884(13) . 1_554
Al8 Co1 Al8 110.21(3) . 1_554
Al6 Co1 Al7 122.25(5) . 7_665
Al8 Co1 Al7 71.59(2) . 7_665
Al8 Co1 Al7 71.59(2) 1_554 7_665
Al6 Co1 Al7 124.79(6) . 3_455
Al8 Co1 Al7 71.59(2) . 3_455
Al8 Co1 Al7 71.59(2) 1_554 3_455
Al7 Co1 Al7 112.97(4) 7_665 3_455
Al6 Co1 Al5 70.74(4) . 3_455
Al8 Co1 Al5 146.64(4) . 3_455
Al8 Co1 Al5 63.61(3) 1_554 3_455
Al7 Co1 Al5 128.73(3) 7_665 3_455
Al7 Co1 Al5 75.62(4) 3_455 3_455
Al6 Co1 Al5 70.74(4) . 3_456
Al8 Co1 Al5 63.61(3) . 3_456
Al8 Co1 Al5 146.64(4) 1_554 3_456
Al7 Co1 Al5 128.73(3) 7_665 3_456
Al7 Co1 Al5 75.62(4) 3_455 3_456
Al5 Co1 Al5 102.54(5) 3_455 3_456
Al6 Co1 Al2 69.80(4) . .
Al8 Co1 Al2 63.33(3) . .
Al8 Co1 Al2 146.15(4) 1_554 .
Al7 Co1 Al2 75.09(4) 7_665 .
Al7 Co1 Al2 128.74(3) 3_455 .
Al5 Co1 Al2 140.54(5) 3_455 .
Al5 Co1 Al2 63.59(4) 3_456 .
Al6 Co1 Al2 69.80(4) . 1_554
Al8 Co1 Al2 146.15(4) . 1_554
Al8 Co1 Al2 63.33(3) 1_554 1_554
Al7 Co1 Al2 75.09(4) 7_665 1_554
Al7 Co1 Al2 128.74(3) 3_455 1_554
Al5 Co1 Al2 63.59(4) 3_455 1_554
Al5 Co1 Al2 140.54(5) 3_456 1_554
Al2 Co1 Al2 102.50(5) . 1_554
Al6 Co1 Mn1 178.73(6) . 5_565
Al8 Co1 Mn1 55.106(13) . 5_565
Al8 Co1 Mn1 55.107(13) 1_554 5_565
Al7 Co1 Mn1 56.49(4) 7_665 5_565
Al7 Co1 Mn1 56.48(4) 3_455 5_565
Al5 Co1 Mn1 109.97(4) 3_455 5_565
Al5 Co1 Mn1 109.97(4) 3_456 5_565
Al2 Co1 Mn1 109.49(4) . 5_565
Al2 Co1 Mn1 109.49(4) 1_554 5_565
Al6 Co1 Co1 178.73(6) . 5_565
Al8 Co1 Co1 55.106(13) . 5_565
Al8 Co1 Co1 55.107(13) 1_554 5_565
Al7 Co1 Co1 56.49(4) 7_665 5_565
Al7 Co1 Co1 56.48(4) 3_455 5_565
Al5 Co1 Co1 109.97(4) 3_455 5_565
Al5 Co1 Co1 109.97(4) 3_456 5_565
Al2 Co1 Co1 109.49(4) . 5_565
Al2 Co1 Co1 109.49(4) 1_554 5_565
Mn1 Co1 Co1 0.00(3) 5_565 5_565
Al9 Co2 Al6 109.43(4) . .
Al9 Co2 Al7 125.66(4) . .
Al6 Co2 Al7 124.91(6) . .
Al9 Co2 Al3 126.44(3) . .
Al6 Co2 Al3 73.13(4) . .
Al7 Co2 Al3 74.55(4) . .
Al9 Co2 Al3 126.44(3) . 1_554
Al6 Co2 Al3 73.13(4) . 1_554
Al7 Co2 Al3 74.55(4) . 1_554
Al3 Co2 Al3 105.98(6) . 1_554
Al9 Co2 Al4 73.28(4) . 7_654
Al6 Co2 Al4 126.70(3) . 7_654
Al7 Co2 Al4 74.65(4) . 7_654
Al3 Co2 Al4 149.20(5) . 7_654
Al3 Co2 Al4 65.63(4) 1_554 7_654
Al9 Co2 Al4 73.28(4) . 7_655
Al6 Co2 Al4 126.70(3) . 7_655
Al7 Co2 Al4 74.65(4) . 7_655
Al3 Co2 Al4 65.63(4) . 7_655
Al3 Co2 Al4 149.20(5) 1_554 7_655
Al4 Co2 Al4 105.53(6) 7_654 7_655
Al9 Co2 Al1 68.34(3) . 1_554
Al6 Co2 Al1 68.84(4) . 1_554
Al7 Co2 Al1 129.19(3) . 1_554
Al3 Co2 Al1 141.97(5) . 1_554
Al3 Co2 Al1 63.25(4) 1_554 1_554
Al4 Co2 Al1 63.24(4) 7_654 1_554
Al4 Co2 Al1 141.62(5) 7_655 1_554
Al9 Co2 Al1 68.34(3) . .
Al6 Co2 Al1 68.84(4) . .
Al7 Co2 Al1 129.19(3) . .
Al3 Co2 Al1 63.25(4) . .
Al3 Co2 Al1 141.97(5) 1_554 .
Al4 Co2 Al1 141.62(5) 7_654 .
Al4 Co2 Al1 63.24(4) 7_655 .
Al1 Co2 Al1 101.62(5) 1_554 .
Mn2 Al1 Co2 0.00(3) 1_556 1_556
Mn2 Al1 Co2 101.62(5) 1_556 .
Co2 Al1 Co2 101.62(5) 1_556 .
Mn2 Al1 Al3 56.99(3) 1_556 .
Co2 Al1 Al3 56.99(3) 1_556 .
Co2 Al1 Al3 56.99(3) . .
Mn2 Al1 Al4 57.13(3) 1_556 7_655
Co2 Al1 Al4 57.13(3) 1_556 7_655
Co2 Al1 Al4 57.13(3) . 7_655
Al3 Al1 Al4 61.24(5) . 7_655
Mn2 Al1 Al9 119.91(5) 1_556 .
Co2 Al1 Al9 119.91(5) 1_556 .
Co2 Al1 Al9 51.47(2) . .
Al3 Al1 Al9 105.15(4) . .
Al4 Al1 Al9 64.26(3) 7_655 .
Mn2 Al1 Al9 51.47(2) 1_556 1_556
Co2 Al1 Al9 51.47(2) 1_556 1_556
Co2 Al1 Al9 119.91(5) . 1_556
Al3 Al1 Al9 105.15(4) . 1_556
Al4 Al1 Al9 64.26(3) 7_655 1_556
Al9 Al1 Al9 92.70(4) . 1_556
Mn2 Al1 Al6 51.43(3) 1_556 1_556
Co2 Al1 Al6 51.43(3) 1_556 1_556
Co2 Al1 Al6 119.28(6) . 1_556
Al3 Al1 Al6 63.88(4) . 1_556
Al4 Al1 Al6 105.13(5) 7_655 1_556
Al9 Al1 Al6 168.24(6) . 1_556
Al9 Al1 Al6 86.58(2) 1_556 1_556
Mn2 Al1 Al6 119.28(6) 1_556 .
Co2 Al1 Al6 119.28(6) 1_556 .
Co2 Al1 Al6 51.43(3) . .
Al3 Al1 Al6 63.88(4) . .
Al4 Al1 Al6 105.13(5) 7_655 .
Al9 Al1 Al6 86.58(2) . .
Al9 Al1 Al6 168.24(6) 1_556 .
Al6 Al1 Al6 91.74(6) 1_556 .
Mn2 Al1 Al5 111.96(4) 1_556 3_456
Co2 Al1 Al5 111.96(4) 1_556 3_456
Co2 Al1 Al5 111.96(4) . 3_456
Al3 Al1 Al5 95.85(6) . 3_456
Al4 Al1 Al5 157.09(7) 7_655 3_456
Al9 Al1 Al5 127.51(3) . 3_456
Al9 Al1 Al5 127.51(3) 1_556 3_456
Al6 Al1 Al5 60.54(4) 1_556 3_456
Al6 Al1 Al5 60.54(4) . 3_456
Mn2 Al1 Ce1 169.01(4) 1_556 3_455
Co2 Al1 Ce1 169.01(4) 1_556 3_455
Co2 Al1 Ce1 89.363(15) . 3_455
Al3 Al1 Ce1 131.67(4) . 3_455
Al4 Al1 Ce1 131.06(4) 7_655 3_455
Al9 Al1 Ce1 66.945(19) . 3_455
Al9 Al1 Ce1 122.36(5) 1_556 3_455
Al6 Al1 Ce1 123.03(5) 1_556 3_455
Al6 Al1 Ce1 68.02(3) . 3_455
Al5 Al1 Ce1 63.25(3) 3_456 3_455
Co1 Al2 Mn1 102.50(5) . 1_556
Co1 Al2 Co1 102.50(5) . 1_556
Mn1 Al2 Co1 0.00(2) 1_556 1_556
Co1 Al2 Al8 55.99(3) . .
Mn1 Al2 Al8 55.99(3) 1_556 .
Co1 Al2 Al8 55.99(3) 1_556 .
Co1 Al2 Al4 112.90(4) . .
Mn1 Al2 Al4 112.90(4) 1_556 .
Co1 Al2 Al4 112.90(4) 1_556 .
Al8 Al2 Al4 101.77(6) . .
Co1 Al2 Al5 58.19(3) . 3_456
Mn1 Al2 Al5 58.19(3) 1_556 3_456
Co1 Al2 Al5 58.19(3) 1_556 3_456
Al8 Al2 Al5 59.32(4) . 3_456
Al4 Al2 Al5 161.08(7) . 3_456
Co1 Al2 Al6 51.07(3) . .
Mn1 Al2 Al6 118.95(6) 1_556 .
Co1 Al2 Al6 118.95(6) 1_556 .
Al8 Al2 Al6 101.97(5) . .
Al4 Al2 Al6 127.82(4) . .
Al5 Al2 Al6 61.97(4) 3_456 .
Co1 Al2 Al6 118.95(6) . 1_556
Mn1 Al2 Al6 51.07(3) 1_556 1_556
Co1 Al2 Al6 51.07(3) 1_556 1_556
Al8 Al2 Al6 101.97(5) . 1_556
Al4 Al2 Al6 127.82(4) . 1_556
Al5 Al2 Al6 61.97(4) 3_456 1_556
Al6 Al2 Al6 91.01(6) . 1_556
Co1 Al2 Ce1 167.63(5) . 1_556
Mn1 Al2 Ce1 88.816(16) 1_556 1_556
Co1 Al2 Ce1 88.816(16) 1_556 1_556
Al8 Al2 Ce1 136.22(3) . 1_556
Al4 Al2 Ce1 66.05(4) . 1_556
Al5 Al2 Ce1 126.56(4) 3_456 1_556
Al6 Al2 Ce1 118.90(5) . 1_556
Al6 Al2 Ce1 64.60(3) 1_556 1_556
Co1 Al2 Ce1 88.816(16) . .
Mn1 Al2 Ce1 167.63(5) 1_556 .
Co1 Al2 Ce1 167.63(5) 1_556 .
Al8 Al2 Ce1 136.22(3) . .
Al4 Al2 Ce1 66.05(4) . .
Al5 Al2 Ce1 126.56(4) 3_456 .
Al6 Al2 Ce1 64.60(3) . .
Al6 Al2 Ce1 118.90(5) 1_556 .
Ce1 Al2 Ce1 79.51(3) 1_556 .
Co2 Al3 Mn2 105.98(6) . 1_556
Co2 Al3 Co2 105.98(6) . 1_556
Mn2 Al3 Co2 0.00(4) 1_556 1_556
Co2 Al3 Al1 59.76(3) . .
Mn2 Al3 Al1 59.76(3) 1_556 .
Co2 Al3 Al1 59.76(3) 1_556 .
Co2 Al3 Al5 115.77(4) . .
Mn2 Al3 Al5 115.77(4) 1_556 .
Co2 Al3 Al5 115.77(4) 1_556 .
Al1 Al3 Al5 169.45(7) . .
Co2 Al3 Al4 57.31(3) . 7_655
Mn2 Al3 Al4 57.31(3) 1_556 7_655
Co2 Al3 Al4 57.31(3) 1_556 7_655
Al1 Al3 Al4 59.44(5) . 7_655
Al5 Al3 Al4 110.02(6) . 7_655
Co2 Al3 Al6 50.74(3) . .
Mn2 Al3 Al6 118.27(6) 1_556 .
Co2 Al3 Al6 118.27(6) 1_556 .
Al1 Al3 Al6 60.07(4) . .
Al5 Al3 Al6 125.86(4) . .
Al4 Al3 Al6 101.22(5) 7_655 .
Co2 Al3 Al6 118.27(6) . 1_556
Mn2 Al3 Al6 50.74(3) 1_556 1_556
Co2 Al3 Al6 50.74(3) 1_556 1_556
Al1 Al3 Al6 60.07(4) . 1_556
Al5 Al3 Al6 125.86(4) . 1_556
Al4 Al3 Al6 101.22(5) 7_655 1_556
Al6 Al3 Al6 87.70(6) . 1_556
Co2 Al3 Ce1 163.93(5) . 1_556
Mn2 Al3 Ce1 87.273(17) 1_556 1_556
Co2 Al3 Ce1 87.273(17) 1_556 1_556
Al1 Al3 Ce1 123.15(4) . 1_556
Al5 Al3 Ce1 64.10(3) . 1_556
Al4 Al3 Ce1 138.72(2) 7_655 1_556
Al6 Al3 Ce1 115.09(5) . 1_556
Al6 Al3 Ce1 63.20(3) 1_556 1_556
Co2 Al3 Ce1 87.273(17) . .
Mn2 Al3 Ce1 163.93(5) 1_556 .
Co2 Al3 Ce1 163.93(5) 1_556 .
Al1 Al3 Ce1 123.15(4) . .
Al5 Al3 Ce1 64.10(3) . .
Al4 Al3 Ce1 138.72(2) 7_655 .
Al6 Al3 Ce1 63.20(3) . .
Al6 Al3 Ce1 115.09(5) 1_556 .
Ce1 Al3 Ce1 78.32(3) 1_556 .
Mn2 Al4 Co2 0.0 7_666 7_666
Mn2 Al4 Mn2 105.53(6) 7_666 7_665
Co2 Al4 Mn2 105.53(6) 7_666 7_665
Mn2 Al4 Co2 105.53(6) 7_666 7_665
Co2 Al4 Co2 105.53(6) 7_666 7_665
Mn2 Al4 Co2 0.00(2) 7_665 7_665
Mn2 Al4 Al1 59.63(3) 7_666 7_665
Co2 Al4 Al1 59.63(3) 7_666 7_665
Mn2 Al4 Al1 59.63(3) 7_665 7_665
Co2 Al4 Al1 59.63(3) 7_665 7_665
Mn2 Al4 Al2 115.44(4) 7_666 .
Co2 Al4 Al2 115.44(4) 7_666 .
Mn2 Al4 Al2 115.44(4) 7_665 .
Co2 Al4 Al2 115.44(4) 7_665 .
Al1 Al4 Al2 168.55(7) 7_665 .
Mn2 Al4 Al3 57.05(3) 7_666 7_665
Co2 Al4 Al3 57.05(3) 7_666 7_665
Mn2 Al4 Al3 57.05(3) 7_665 7_665
Co2 Al4 Al3 57.05(3) 7_665 7_665
Al1 Al4 Al3 59.32(5) 7_665 7_665
Al2 Al4 Al3 109.23(7) . 7_665
Mn2 Al4 Al9 50.41(2) 7_666 3_556
Co2 Al4 Al9 50.41(2) 7_666 3_556
Mn2 Al4 Al9 117.66(5) 7_665 3_556
Co2 Al4 Al9 117.66(5) 7_665 3_556
Al1 Al4 Al9 59.44(3) 7_665 3_556
Al2 Al4 Al9 126.88(4) . 3_556
Al3 Al4 Al9 100.47(4) 7_665 3_556
Mn2 Al4 Al9 117.66(5) 7_666 3
Co2 Al4 Al9 117.66(5) 7_666 3
Mn2 Al4 Al9 50.41(2) 7_665 3
Co2 Al4 Al9 50.41(2) 7_665 3
Al1 Al4 Al9 59.44(3) 7_665 3
Al2 Al4 Al9 126.88(4) . 3
Al3 Al4 Al9 100.47(4) 7_665 3
Al9 Al4 Al9 87.54(4) 3_556 3
Mn2 Al4 Ce1 164.30(5) 7_666 .
Co2 Al4 Ce1 164.30(5) 7_666 .
Mn2 Al4 Ce1 87.861(17) 7_665 .
Co2 Al4 Ce1 87.861(17) 7_665 .
Al1 Al4 Ce1 124.02(4) 7_665 .
Al2 Al4 Ce1 63.83(3) . .
Al3 Al4 Ce1 138.65(3) 7_665 .
Al9 Al4 Ce1 116.20(5) 3_556 .
Al9 Al4 Ce1 64.699(19) 3 .
Mn2 Al4 Ce1 87.861(17) 7_666 1_556
Co2 Al4 Ce1 87.861(17) 7_666 1_556
Mn2 Al4 Ce1 164.30(5) 7_665 1_556
Co2 Al4 Ce1 164.30(5) 7_665 1_556
Al1 Al4 Ce1 124.02(4) 7_665 1_556
Al2 Al4 Ce1 63.83(3) . 1_556
Al3 Al4 Ce1 138.65(3) 7_665 1_556
Al9 Al4 Ce1 64.699(19) 3_556 1_556
Al9 Al4 Ce1 116.20(5) 3 1_556
Ce1 Al4 Ce1 77.81(3) . 1_556
Mn1 Al5 Co1 0.00(4) 3 3
Mn1 Al5 Mn1 102.54(5) 3 3_556
Co1 Al5 Mn1 102.54(5) 3 3_556
Mn1 Al5 Co1 102.54(5) 3 3_556
Co1 Al5 Co1 102.54(5) 3 3_556
Mn1 Al5 Co1 0.00(3) 3_556 3_556
Mn1 Al5 Al8 55.88(3) 3 3_556
Co1 Al5 Al8 55.88(3) 3 3_556
Mn1 Al5 Al8 55.88(3) 3_556 3_556
Co1 Al5 Al8 55.88(3) 3_556 3_556
Mn1 Al5 Al3 112.12(4) 3 .
Co1 Al5 Al3 112.12(4) 3 .
Mn1 Al5 Al3 112.12(4) 3_556 .
Co1 Al5 Al3 112.12(4) 3_556 .
Al8 Al5 Al3 100.72(5) 3_556 .
Mn1 Al5 Al2 58.22(3) 3 3_556
Co1 Al5 Al2 58.22(3) 3 3_556
Mn1 Al5 Al2 58.22(3) 3_556 3_556
Co1 Al5 Al2 58.22(3) 3_556 3_556
Al8 Al5 Al2 58.95(4) 3_556 3_556
Al3 Al5 Al2 159.67(7) . 3_556
Mn1 Al5 Al6 117.81(6) 3 3_556
Co1 Al5 Al6 117.81(6) 3 3_556
Mn1 Al5 Al6 50.68(3) 3_556 3_556
Co1 Al5 Al6 50.68(3) 3_556 3_556
Al8 Al5 Al6 100.88(5) 3_556 3_556
Al3 Al5 Al6 129.52(4) . 3_556
Al2 Al5 Al6 60.78(4) 3_556 3_556
Mn1 Al5 Al6 50.68(3) 3 3
Co1 Al5 Al6 50.68(3) 3 3
Mn1 Al5 Al6 117.81(6) 3_556 3
Co1 Al5 Al6 117.81(6) 3_556 3
Al8 Al5 Al6 100.88(5) 3_556 3
Al3 Al5 Al6 129.52(4) . 3
Al2 Al5 Al6 60.78(4) 3_556 3
Al6 Al5 Al6 89.70(6) 3_556 3
Mn1 Al5 Al1 109.49(4) 3 3_556
Co1 Al5 Al1 109.49(4) 3 3_556
Mn1 Al5 Al1 109.49(4) 3_556 3_556
Co1 Al5 Al1 109.49(4) 3_556 3_556
Al8 Al5 Al1 148.52(6) 3_556 3_556
Al3 Al5 Al1 110.76(6) . 3_556
Al2 Al5 Al1 89.57(6) 3_556 3_556
Al6 Al5 Al1 58.82(4) 3_556 3_556
Al6 Al5 Al1 58.82(4) 3 3_556
Mn1 Al5 Ce1 168.01(4) 3 1_556
Co1 Al5 Ce1 168.01(4) 3 1_556
Mn1 Al5 Ce1 89.022(16) 3_556 1_556
Co1 Al5 Ce1 89.022(16) 3_556 1_556
Al8 Al5 Ce1 135.52(3) 3_556 1_556
Al3 Al5 Ce1 65.32(3) . 1_556
Al2 Al5 Ce1 128.05(4) 3_556 1_556
Al6 Al5 Ce1 67.27(3) 3_556 1_556
Al6 Al5 Ce1 120.89(5) 3 1_556
Al1 Al5 Ce1 62.80(3) 3_556 1_556
Mn1 Al5 Ce1 89.022(16) 3 .
Co1 Al5 Ce1 89.022(16) 3 .
Mn1 Al5 Ce1 168.01(4) 3_556 .
Co1 Al5 Ce1 168.01(4) 3_556 .
Al8 Al5 Ce1 135.52(3) 3_556 .
Al3 Al5 Ce1 65.32(3) . .
Al2 Al5 Ce1 128.05(4) 3_556 .
Al6 Al5 Ce1 120.89(5) 3_556 .
Al6 Al5 Ce1 67.27(3) 3 .
Al1 Al5 Ce1 62.80(3) 3_556 .
Ce1 Al5 Ce1 79.27(3) 1_556 .
Co1 Al6 Co2 178.14(7) . .
Co1 Al6 Al1 119.23(5) . 1_554
Co2 Al6 Al1 59.73(4) . 1_554
Co1 Al6 Al1 119.23(5) . .
Co2 Al6 Al1 59.73(4) . .
Al1 Al6 Al1 91.74(6) 1_554 .
Co1 Al6 Al2 59.13(4) . .
Co2 Al6 Al2 121.89(4) . .
Al1 Al6 Al2 178.20(7) 1_554 .
Al1 Al6 Al2 88.60(3) . .
Co1 Al6 Al2 59.13(4) . 1_554
Co2 Al6 Al2 121.89(4) . 1_554
Al1 Al6 Al2 88.60(3) 1_554 1_554
Al1 Al6 Al2 178.20(7) . 1_554
Al2 Al6 Al2 91.01(6) . 1_554
Co1 Al6 Al5 58.59(4) . 3_455
Co2 Al6 Al5 120.36(4) . 3_455
Al1 Al6 Al5 60.64(4) 1_554 3_455
Al1 Al6 Al5 121.47(6) . 3_455
Al2 Al6 Al5 117.72(6) . 3_455
Al2 Al6 Al5 57.25(4) 1_554 3_455
Co1 Al6 Al5 58.59(4) . 3_456
Co2 Al6 Al5 120.36(4) . 3_456
Al1 Al6 Al5 121.47(6) 1_554 3_456
Al1 Al6 Al5 60.64(4) . 3_456
Al2 Al6 Al5 57.25(4) . 3_456
Al2 Al6 Al5 117.72(6) 1_554 3_456
Al5 Al6 Al5 89.70(6) 3_455 3_456
Co1 Al6 Al3 124.88(4) . .
Co2 Al6 Al3 56.12(4) . .
Al1 Al6 Al3 115.85(6) 1_554 .
Al1 Al6 Al3 56.05(4) . .
Al2 Al6 Al3 65.76(4) . .
Al2 Al6 Al3 125.30(6) 1_554 .
Al5 Al6 Al3 176.19(7) 3_455 .
Al5 Al6 Al3 91.18(3) 3_456 .
Co1 Al6 Al3 124.88(4) . 1_554
Co2 Al6 Al3 56.12(4) . 1_554
Al1 Al6 Al3 56.05(4) 1_554 1_554
Al1 Al6 Al3 115.85(6) . 1_554
Al2 Al6 Al3 125.30(6) . 1_554
Al2 Al6 Al3 65.76(4) 1_554 1_554
Al5 Al6 Al3 91.18(3) 3_455 1_554
Al5 Al6 Al3 176.19(7) 3_456 1_554
Al3 Al6 Al3 87.70(6) . 1_554
Co2 Al7 Mn1 146.55(7) . 7_655
Co2 Al7 Co1 146.55(7) . 7_655
Mn1 Al7 Co1 0.00(3) 7_655 7_655
Co2 Al7 Co1 146.42(7) . 3
Mn1 Al7 Co1 67.03(4) 7_655 3
Co1 Al7 Co1 67.03(4) 7_655 3
Co2 Al7 Mn1 146.42(7) . 3
Mn1 Al7 Mn1 67.03(4) 7_655 3
Co1 Al7 Mn1 67.03(4) 7_655 3
Co1 Al7 Mn1 0.00(3) 3 3
Co2 Al7 Al8 136.480(19) . 3_556
Mn1 Al7 Al8 52.80(2) 7_655 3_556
Co1 Al7 Al8 52.80(2) 7_655 3_556
Co1 Al7 Al8 52.80(2) 3 3_556
Mn1 Al7 Al8 52.80(2) 3 3_556
Co2 Al7 Al8 136.480(19) . 3
Mn1 Al7 Al8 52.80(2) 7_655 3
Co1 Al7 Al8 52.80(2) 7_655 3
Co1 Al7 Al8 52.80(2) 3 3
Mn1 Al7 Al8 52.80(2) 3 3
Al8 Al7 Al8 87.04(4) 3_556 3
Co1 Al8 Mn1 180.0 . 5_566
Co1 Al8 Mn1 110.21(3) . 1_556
Mn1 Al8 Mn1 69.79(3) 5_566 1_556
Co1 Al8 Co1 110.21(3) . 1_556
Mn1 Al8 Co1 69.79(3) 5_566 1_556
Mn1 Al8 Co1 0.00(3) 1_556 1_556
Co1 Al8 Co1 180.0 . 5_566
Mn1 Al8 Co1 0.00(3) 5_566 5_566
Mn1 Al8 Co1 69.79(3) 1_556 5_566
Co1 Al8 Co1 69.79(3) 1_556 5_566
Co1 Al8 Mn1 69.79(3) . 5_565
Mn1 Al8 Mn1 110.21(3) 5_566 5_565
Mn1 Al8 Mn1 180.0 1_556 5_565
Co1 Al8 Mn1 180.0 1_556 5_565
Co1 Al8 Mn1 110.21(3) 5_566 5_565
Co1 Al8 Co1 69.79(3) . 5_565
Mn1 Al8 Co1 110.21(3) 5_566 5_565
Mn1 Al8 Co1 180.0 1_556 5_565
Co1 Al8 Co1 180.0 1_556 5_565
Co1 Al8 Co1 110.21(3) 5_566 5_565
Mn1 Al8 Co1 0.00(4) 5_565 5_565
Co1 Al8 Al2 119.326(17) . 5_566
Mn1 Al8 Al2 60.674(17) 5_566 5_566
Mn1 Al8 Al2 119.326(17) 1_556 5_566
Co1 Al8 Al2 119.326(17) 1_556 5_566
Co1 Al8 Al2 60.674(17) 5_566 5_566
Mn1 Al8 Al2 60.674(17) 5_565 5_566
Co1 Al8 Al2 60.674(17) 5_565 5_566
Co1 Al8 Al2 60.674(17) . .
Mn1 Al8 Al2 119.326(17) 5_566 .
Mn1 Al8 Al2 60.674(17) 1_556 .
Co1 Al8 Al2 60.674(17) 1_556 .
Co1 Al8 Al2 119.326(17) 5_566 .
Mn1 Al8 Al2 119.326(17) 5_565 .
Co1 Al8 Al2 119.326(17) 5_565 .
Al2 Al8 Al2 180.0 5_566 .
Co1 Al8 Al5 60.509(17) . 3_456
Mn1 Al8 Al5 119.491(17) 5_566 3_456
Mn1 Al8 Al5 60.509(17) 1_556 3_456
Co1 Al8 Al5 60.509(17) 1_556 3_456
Co1 Al8 Al5 119.491(17) 5_566 3_456
Mn1 Al8 Al5 119.491(17) 5_565 3_456
Co1 Al8 Al5 119.491(17) 5_565 3_456
Al2 Al8 Al5 118.27(4) 5_566 3_456
Al2 Al8 Al5 61.73(4) . 3_456
Co1 Al8 Al5 119.491(17) . 7_665
Mn1 Al8 Al5 60.509(17) 5_566 7_665
Mn1 Al8 Al5 119.491(17) 1_556 7_665
Co1 Al8 Al5 119.491(17) 1_556 7_665
Co1 Al8 Al5 60.509(17) 5_566 7_665
Mn1 Al8 Al5 60.509(17) 5_565 7_665
Co1 Al8 Al5 60.509(17) 5_565 7_665
Al2 Al8 Al5 61.73(4) 5_566 7_665
Al2 Al8 Al5 118.27(4) . 7_665
Al5 Al8 Al5 180.0 3_456 7_665
Co2 Al9 Mn2 180.00(3) . 5
Co2 Al9 Co2 180.00(3) . 5
Mn2 Al9 Co2 0.00(3) 5 5
Co2 Al9 Al1 119.81(3) . 5
Mn2 Al9 Al1 60.19(3) 5 5
Co2 Al9 Al1 60.19(3) 5 5
Co2 Al9 Al1 60.19(3) . .
Mn2 Al9 Al1 119.81(3) 5 .
Co2 Al9 Al1 119.81(3) 5 .
Al1 Al9 Al1 180.00(7) 5 .
Co2 Al9 Al1 119.81(3) . 5_556
Mn2 Al9 Al1 60.19(3) 5 5_556
Co2 Al9 Al1 60.19(3) 5 5_556
Al1 Al9 Al1 92.70(4) 5 5_556
Al1 Al9 Al1 87.30(4) . 5_556
Co2 Al9 Al1 60.19(3) . 1_554
Mn2 Al9 Al1 119.81(3) 5 1_554
Co2 Al9 Al1 119.81(3) 5 1_554
Al1 Al9 Al1 87.30(4) 5 1_554
Al1 Al9 Al1 92.70(4) . 1_554
Al1 Al9 Al1 180.00(4) 5_556 1_554
Co2 Al9 Al4 123.69(3) . 3_455
Mn2 Al9 Al4 56.31(3) 5 3_455
Co2 Al9 Al4 56.31(3) 5 3_455
Al1 Al9 Al4 56.30(4) 5 3_455
Al1 Al9 Al4 123.70(4) . 3_455
Al1 Al9 Al4 116.50(4) 5_556 3_455
Al1 Al9 Al4 63.50(4) 1_554 3_455
Co2 Al9 Al4 56.31(3) . 7_655
Mn2 Al9 Al4 123.69(3) 5 7_655
Co2 Al9 Al4 123.69(3) 5 7_655
Al1 Al9 Al4 123.70(4) 5 7_655
Al1 Al9 Al4 56.30(4) . 7_655
Al1 Al9 Al4 63.50(4) 5_556 7_655
Al1 Al9 Al4 116.50(4) 1_554 7_655
Al4 Al9 Al4 180.00(7) 3_455 7_655
Co2 Al9 Al4 123.69(3) . 3_456
Mn2 Al9 Al4 56.31(3) 5 3_456
Co2 Al9 Al4 56.31(3) 5 3_456
Al1 Al9 Al4 116.50(4) 5 3_456
Al1 Al9 Al4 63.50(4) . 3_456
Al1 Al9 Al4 56.30(4) 5_556 3_456
Al1 Al9 Al4 123.70(4) 1_554 3_456
Al4 Al9 Al4 87.54(4) 3_455 3_456
Al4 Al9 Al4 92.46(4) 7_655 3_456
Co2 Al9 Al4 56.31(3) . 7_654
Mn2 Al9 Al4 123.69(3) 5 7_654
Co2 Al9 Al4 123.69(3) 5 7_654
Al1 Al9 Al4 63.50(4) 5 7_654
Al1 Al9 Al4 116.50(4) . 7_654
Al1 Al9 Al4 123.70(4) 5_556 7_654
Al1 Al9 Al4 56.30(4) 1_554 7_654
Al4 Al9 Al4 92.46(4) 3_455 7_654
Al4 Al9 Al4 87.54(4) 7_655 7_654
Al4 Al9 Al4 180.00(4) 3_456 7_654
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ce1 Al1 3.1493(11) 3_556
Ce1 Al1 3.1493(11) 3
Ce1 Al2 3.1541(11) 1_554
Ce1 Al2 3.1541(11) .
Ce1 Al5 3.1620(11) .
Ce1 Al5 3.1620(11) 1_554
Ce1 Al3 3.1941(11) 1_554
Ce1 Al3 3.1941(11) .
Ce1 Al6 3.2082(14) .
Ce1 Al4 3.2118(11) .
Ce1 Al4 3.2118(11) 1_554
Ce1 Al9 3.2883(3) 3
Co1 Al6 2.3437(15) .
Co1 Al8 2.4591(4) .
Co1 Al8 2.4591(4) 1_554
Co1 Al7 2.5476(16) 7_665
Co1 Al7 2.5477(15) 3_455
Co1 Al5 2.5856(10) 3_455
Co1 Al5 2.5856(10) 3_456
Co1 Al2 2.5863(10) .
Co1 Al2 2.5863(10) 1_554
Co1 Mn1 2.8135(13) 5_565
Co1 Co1 2.8135(13) 5_565
Co2 Al9 2.3462(6) .
Co2 Al6 2.3558(15) .
Co2 Al7 2.4592(16) .
Co2 Al3 2.5259(10) .
Co2 Al3 2.5259(10) 1_554
Co2 Al4 2.5334(10) 7_654
Co2 Al4 2.5334(10) 7_655
Co2 Al1 2.6024(10) 1_554
Co2 Al1 2.6024(10) .
Al1 Mn2 2.6024(10) 1_556
Al1 Co2 2.6024(10) 1_556
Al1 Al3 2.690(2) .
Al1 Al4 2.693(2) 7_655
Al1 Al9 2.7875(10) .
Al1 Al9 2.7875(10) 1_556
Al1 Al6 2.8101(14) 1_556
Al1 Al6 2.8101(14) .
Al1 Al5 2.863(2) 3_456
Al1 Ce1 3.1493(11) 3_455
Al2 Mn1 2.5863(10) 1_556
Al2 Co1 2.5863(10) 1_556
Al2 Al8 2.6509(14) .
Al2 Al4 2.697(2) .
Al2 Al5 2.725(2) 3_456
Al2 Al6 2.8278(14) .
Al2 Al6 2.8278(14) 1_556
Al2 Ce1 3.1541(11) 1_556
Al3 Mn2 2.5259(10) 1_556
Al3 Co2 2.5259(10) 1_556
Al3 Al5 2.716(2) .
Al3 Al4 2.742(2) 7_655
Al3 Al6 2.9115(15) .
Al3 Al6 2.9115(15) 1_556
Al3 Ce1 3.1941(11) 1_556
Al4 Mn2 2.5334(10) 7_666
Al4 Co2 2.5334(10) 7_666
Al4 Mn2 2.5334(10) 7_665
Al4 Co2 2.5334(10) 7_665
Al4 Al1 2.693(2) 7_665
Al4 Al3 2.742(2) 7_665
Al4 Al9 2.9158(11) 3_556
Al4 Al9 2.9158(11) 3
Al4 Ce1 3.2118(11) 1_556
Al5 Mn1 2.5856(10) 3
Al5 Co1 2.5856(10) 3
Al5 Mn1 2.5856(10) 3_556
Al5 Co1 2.5856(10) 3_556
Al5 Al8 2.6609(14) 3_556
Al5 Al2 2.725(2) 3_556
Al5 Al6 2.8601(14) 3_556
Al5 Al6 2.8601(14) 3
Al5 Al1 2.863(2) 3_556
Al5 Ce1 3.1620(11) 1_556
Al6 Al1 2.8101(14) 1_554
Al6 Al2 2.8278(14) 1_554
Al6 Al5 2.8601(14) 3_455
Al6 Al5 2.8601(14) 3_456
Al6 Al3 2.9115(15) 1_554
Al7 Mn1 2.5476(16) 7_655
Al7 Co1 2.5476(16) 7_655
Al7 Co1 2.5477(15) 3
Al7 Mn1 2.5477(15) 3
Al7 Al8 2.9291(10) 3_556
Al7 Al8 2.9291(10) 3
Al8 Mn1 2.4591(4) 5_566
Al8 Mn1 2.4591(4) 1_556
Al8 Co1 2.4591(4) 1_556
Al8 Co1 2.4591(4) 5_566
Al8 Mn1 2.4591(4) 5_565
Al8 Co1 2.4591(4) 5_565
Al8 Al2 2.6509(14) 5_566
Al8 Al5 2.6609(14) 3_456
Al8 Al5 2.6609(14) 7_665
Al9 Mn2 2.3462(6) 5
Al9 Co2 2.3462(6) 5
Al9 Al1 2.7875(10) 5
Al9 Al1 2.7875(10) 5_556
Al9 Al1 2.7875(10) 1_554
Al9 Al4 2.9158(11) 3_455
Al9 Al4 2.9158(11) 7_655
Al9 Al4 2.9158(11) 3_456
Al9 Al4 2.9158(11) 7_654
